1 Casting since about 4000 BC… Ancient Greece; bronzestatue casting circa 450BCIron works in early Europe,e.g. cast iron cannons fromEngland circa 1543
2 Outline Sand Casting, Investment Casting, Die Casting Basics and countermeasuresPhase Change, ShrinkageHeat TransferPattern DesignVariations & DevelopmentsEnvironmental Issues
3 Casting Readings; Note: a good heat transfer reference can be found by Kalpakjian, Chapters 10, 11, 12Booothroyd, “Design for Die Casting”Flemings “Heat Flow in Solidification”Note: a good heat transfer reference can be found byProf John Lienhard online
4 Casting Methods Sand Casting Investment Casting Die Casting High Temperature Alloy, Complex Geometry, Rough Surface FinishInvestment CastingHigh Temperature Alloy, Complex Geometry, Moderately Smooth Surface FinishDie CastingHigh Temperature Alloy, Moderate Geometry, Smooth Surface
6 Sand CastingDescription: Tempered sand is packed into wood or metal pattern halves, removed form the pattern, and assembled with or without cores, and metal is poured into resultant cavities. Various core materials can be used. Molds are broken to remove castings. Specialized binders now in use can improve tolerances and surface finish.Metals: Most castable metals.Size Range: Limitation depends on foundry capabilities. Ounces to many tons.Tolerances: Non-Ferrous 1/32 to 6 Add .003 to 3, 3/64 from 3 to 6. Across parting line add .020 to .090 depending on size. (Assumes metal patterns)Surface Finish: Non-Ferrous: RMS Ferrous: RMSMinimum Draft Requirements: 1° to 5° Cores: 1° to 1 1/2°Normal Minimum Section Thickness: Non-Ferrous: 1/8 - 1/4 Ferrous: 1/4 - 3/8Ordering Quantities: All quantitiesNormal Lead Time: Samples: 2-10 weeks Production 2-4 weeks A.S.A.
7 Sand Casting Mold Features Vents, which are placed in molds to carry off gases produced when the molten metal comes into contact with the sand in the molds and core. They also exhaust air from the mold cavity as the molten metal flows into the mold.
10 Investment CastingThe investment-casting process, also called the lost-wax process, was first used during the period B.C. The pattern is made of wax or a plastic such as polystyrene. The sequences involved in investment casting are shown in Figure The pattern is made by injecting molten wax or plastic into a metal die in the shape of the object.
11 Investment CastingDescription: Metal mold makes wax or plastic replica. There are sprued, then surrounded with investment material, baked out, and metal is poured in the resultant cavity. Molds are broken to remove the castings.Metals: Most castable metals.Size Range: fraction of an ounce to 150 lbs..Tolerances: .003 to 1/4 .004 to 1/2, .005 per inch to 3 .003 for each additional inchSurface Finish: RMSMinimum Draft Requirements: NoneNormal Minimum Section Thickness: .030 (Small Areas) .060 (Large Areas)Ordering Quantities: Aluminum: usually under 1,000 Other metals: all quantitiesNormal Lead Time: Samples: 5-16 weeks (depending on complexity) Production 4-12 weeks A.S.A. (depending on subsequent operations).Talbot Associates Inc.
12 Die Casting – Cold-Chamber Casting Cycle in cold-chamber casting: (1) with die closed and ram withdrawn, molten metal is poured into the chamber; (2) ram forces metal to flow into die, maintaining pressure during the cooling and solidification; and (3) ram is withdrawn, die is opened, and part is ejected. Used for higher temperature metals eg Aluminum, Copper and alloys
13 Die Casting – Hot-Chamber Casting Cycle in hot-chamber casting: (1) with die closed and plunger withdrawn, molten metal flows into the chamber; (2) plunger forces metal in chamber to flow into die, maintaining pressure during cooling and solidification; and (3) plunger is withdrawn, die is opened, and solidified part is ejected. Finished part is shown in (4).
14 Die CastingDescription: Molten metal is injected, under pressure, into hardened steel dies, often water cooled. Dies are opened, and castings are ejected.Metals: Aluminum, Zinc, Magnesium, and limited Brass.Size Range: Not normally over 2 feet square. Some foundries capable of larger sizes.Tolerances: Al and Mg .002/in. Zinc .0015/in. Brass .001/in. Add .001 to .015 across parting line depending on sizeSurface Finish: 32-63RMSMinimum Draft Requirements: Al & Mg: 1° to 3° Zinc: 1/2° to 2° Brass: 2° to 5°Normal Minimum Section Thickness: Al & Mg: .03 Small Parts: .06 Medium Parts Zinc: .03 Small Parts: .045 Medium Parts Brass: .025 Small Parts: .040 Medium PartsOrdering Quantities: Usually 2,500 and up.Normal Lead Time: Samples: weeks Production: ASAP after approval.
15 High Melt Temperature Chemical Activity High Latent Heat Handling Off-gassingTungsten Carbide, WC, Silicon Carbide, SiCCubic Zirconia, ZrO2MolybdenumAlumina Al2O3Platinum, Pt Titanium, Ti IronFE, Plain Carbon Steels, low alloy, stainless Nickel, Ni Nickel AllowsSilicon, SiCopper, Cu, Bronze, BrassAluminum Magnesium Zinc, Zn PTFE (Teflon) Tin, Sn HDPENylon Acetal
16 Mold Filling Bernouli’s Equation: h Reynold’s Number: Short filling timesPotential Turbulence(see p. 273 … Kalpakjian
41 And more…Figure Omit outside bosses and the need for cores. (Courtesy of Meehanite Metal Corp.)Figure Avoid using ribs which meet at acute angles. (Courtesy of Meehanite Metal Corp.)
42 Die Casting Solidification Time Time to formsolid partA
43 Time to cool part to the ejection temperature. (lumped parameter model) Integration yields…letOr for thin sheets of thickness “w”,Di = Ti + DTsp - TmoldDTsp = H/CpDf = Teject - Tmold“sp” means superheat
45 Pattern DesignTable 12.1Normal Shrinkage Allowance for Some Metals Cast in Sand MoldsMetal PercentGray cast iron 0.83 – 1.3White cast iron 2.1Malleable cast iron 0.78 – 1.0Aluminum alloys 1.3Magnesium alloys 1.3Yellow brass 1.3 – 1.6Phosphor bronze 1.0 – 1.6Aluminum bronze 2.1High-manganese steel 2.6
46 Variations and Developments Continuous castingLost foam molding3D Printing of Investment toolingDirect printing with metal dropletsUniform metal spray
47 Continuous casting ref AISI Steel from the electric or basic oxygen furnace is tapped into a ladle and taken tothe continuous casting machine. The ladle is raised onto a turret that rotates the ladleinto the casting position above the tundish. Referring to Figure 2, liquid steel flows outof the ladle (1) into the tundish (2), and then into a water-cooled copper mold (3).Solidification begins in the mold, and continues through the First Zone (4) and Strand Guide (5).In this configuration, the strand is straightened (6), torch-cut (8), then discharged (12)for intermediate storage or hot charged for finished rolling.